This article may be too technical for most readers to understand. Please help improve it to make it understandable to non-experts, without removing the technical details. (April 2015) (Learn how and when to remove this template message)
In electromagnetism, the magnetic susceptibility (Latin: susceptibilis, "receptive"; denoted χ) is one measure of the magnetic properties of a material. The susceptibility indicates whether a material is attracted into or repelled out of a magnetic field, which in turn has implications for practical applications. Quantitative measures of the magnetic susceptibility also provide insights into the structure of materials, providing insight into bonding and energy levels.
If the magnetic susceptibility is greater than zero, the substance is said to be "paramagnetic"; the magnetization of the substance is higher than that of empty space. If the magnetic susceptibility is less than zero, the substance is "diamagnetic"; it tends to exclude a magnetic field from its interior. 
Mathematically it is the ratio of magnetization I (magnetic moment per unit volume) to the applied magnetizing field intensity H.
Definition of volume susceptibilityEdit
Magnetic susceptibility is a dimensionless proportionality constant that indicates the degree of magnetization of a material in response to an applied magnetic field. A related term is magnetizability, the proportion between magnetic moment and magnetic flux density. A closely related parameter is the permeability, which expresses the total magnetization of material and volume.
The volume magnetic susceptibility, represented by the symbol (often simply , sometimes – magnetic, to distinguish from the electric susceptibility), is defined in the International System of Units — in other systems there may be additional constants — by the following relationship:
- M is the magnetization of the material (the magnetic dipole moment per unit volume), measured in amperes per meter, and
- H is the magnetic field strength, also measured in amperes per meter.
is therefore a dimensionless quantity.
where μ0 is the vacuum permeability (see table of physical constants), and is the relative permeability of the material. Thus the volume magnetic susceptibility and the magnetic permeability are related by the following formula:
This allows an alternative description of all magnetization phenomena in terms of the quantities I and B, as opposed to the commonly used M and H.
Note that these definitions are according to SI conventions. However, many tables of magnetic susceptibility give CGS values (more specifically emu-cgs, short for electromagnetic units, or Gaussian-cgs; both are the same in this context). These units rely on a different definition of the permeability of free space:
In physics it is common (in older literature) to see CGS mass susceptibility given in emu/g, so to convert to SI volume susceptibility we use the conversion 
where is the density given in g/cm3, or
where is the density given in kg/m3.
Mass susceptibility and molar susceptibilityEdit
There are two other measures of susceptibility, the mass magnetic susceptibility (χmass or χg, sometimes χm), measured in m3·kg−1 in SI or in cm3·g−1 in CGS and the molar magnetic susceptibility (χmol) measured in m3·mol−1 (SI) or cm3·mol−1 (CGS) that are defined below, where ρ is the density in kg·m−3 (SI) or g·cm−3 (CGS) and M is molar mass in kg·mol−1 (SI) or g·mol−1 (CGS).
Sign of susceptibility: diamagnetics and other types of magnetismEdit
If χ is positive, a material can be paramagnetic. In this case, the magnetic field in the material is strengthened by the induced magnetization. Alternatively, if χ is negative, the material is diamagnetic. In this case, the magnetic field in the material is weakened by the induced magnetization. Generally, non-magnetic materials are said to be para- or diamagnetic because they do not possess permanent magnetization without external magnetic field. Ferromagnetic, ferrimagnetic, or antiferromagnetic materials have positive susceptibility and possess permanent magnetization even without external magnetic field.
Experimental methods to determine susceptibilityEdit
Volume magnetic susceptibility is measured by the force change felt upon a substance when a magnetic field gradient is applied. Early measurements are made using the Gouy balance where a sample is hung between the poles of an electromagnet. The change in weight when the electromagnet is turned on is proportional to the susceptibility. Today, high-end measurement systems use a superconductive magnet. An alternative is to measure the force change on a strong compact magnet upon insertion of the sample. This system, widely used today, is called the Evans balance. For liquid samples, the susceptibility can be measured from the dependence of the NMR frequency of the sample on its shape or orientation. Another method using MRI/NMR techniques measures the magnetic field distortion around a sample immersed in water inside an MR scanner. This method is highly accurate for diamagnetic materials with susceptibilities similar to water.
The magnetic susceptibility of most crystals is not a scalar quantity. Magnetic response M is dependent upon the orientation of the sample and can occur in directions other than that of the applied field H. In these cases, volume susceptibility is defined as a tensor
where i and j refer to the directions (e.g., x and y in Cartesian coordinates) of the applied field and magnetization, respectively. The tensor is thus rank 2 (second order), dimension (3,3) describing the component of magnetization in the i-th direction from the external field applied in the j-th direction.
In ferromagnetic crystals, the relationship between M and H is not linear. To accommodate this, a more general definition of differential susceptibility is used
where is a tensor derived from partial derivatives of components of M with respect to components of H. When the coercivity of the material parallel to an applied field is the smaller of the two, the differential susceptibility is a function of the applied field and self interactions, such as the magnetic anisotropy. When the material is not saturated, the effect will be nonlinear and dependent upon the domain wall configuration of the material.
Susceptibility in the frequency domainEdit
When the magnetic susceptibility is measured in response to an AC magnetic field (i.e. a magnetic field that varies sinusoidally), this is called AC susceptibility. AC susceptibility (and the closely related "AC permeability") are complex number quantities, and various phenomena (such as resonances) can be seen in AC susceptibility that cannot in constant-field (DC) susceptibility. In particular, when an AC field is applied perpendicular to the detection direction (called the "transverse susceptibility" regardless of the frequency), the effect has a peak at the ferromagnetic resonance frequency of the material with a given static applied field. Currently, this effect is called the microwave permeability or network ferromagnetic resonance in the literature. These results are sensitive to the domain wall configuration of the material and eddy currents.
In terms of ferromagnetic resonance, the effect of an ac-field applied along the direction of the magnetization is called parallel pumping.
For a tutorial with more information on AC susceptibility measurements, see here (external link).
|Material||Temp.||Pressure||Molar susc.,||Mass susc.,||Volume susc.,||Molar mass, M||Density,|
|Paraffin oil, 220–260 cSt||22||1||−10.1×10−9||−8.0×10−7||−8.8×10−6||−7.0×10−7||0.878|
|Fused silica glass||22||1||−5.12×10−9||−4.07×10−7||−11.28×10−6||−8.98×10−7||2.20|
|Graphite (to c-axis)||R.T.||1||−7.5×10−11||−6.0×10−6||−6.3×10−9||−5.0×10−7||−1.4×10−5||−1.1×10−6||12.01||2.267|
Sources of confusion in published dataEdit
The CRC Handbook of Chemistry and Physics has one of the only published magnetic susceptibility tables. Some of the data (e.g., for Al, Bi, and diamond) is listed as CGS. CGS has caused confusion to some readers. CGS is an abbreviation of centimeters–grams–seconds; it represents the form of the units, but CGS does not specify units. Correct units of magnetic susceptibility in CGS is cm3/mol or cm3/g. Molar susceptibility and mass susceptibility are both listed in the CRC. Some table have listed magnetic susceptibility of diamagnets as positives. It is important to check the header of the table for the correct units and sign of magnetic susceptibility readings.
References and notesEdit
- Roger Grinter, The Quantum in Chemistry: An Experimentalist's View, John Wiley & Sons, 2005, ISBN 0470017627 page 364
- "magnetizability, ξ". IUPAC Compendium of Chemical Terminology—The Gold Book (2nd ed.). International Union of Pure and Applied Chemistry. 1997.
- O'Handley, Robert C. (2000). Modern Magnetic Materials. Hoboken, NJ: Wiley. ISBN 9780471155669.
- Richard A. Clarke. "Magnetic properties of materials". Info.ee.surrey.ac.uk. Retrieved 2011-11-08.
- Bennett, L. H.; Page, C. H. & Swartzendruber, L. J. (1978). "Comments on units in magnetism". Journal of Research of the National Bureau of Standards. NIST, USA. 83 (1): 9–12.
- "IEEE Magnetic unit conversions".
- L. N. Mulay (1972). A. Weissberger; B. W. Rossiter, eds. Techniques of Chemistry. 4. Wiley-Interscience: New York. p. 431.
- "Magnetic Susceptibility Balances". Sherwood-scientific.com. Retrieved 2011-11-08.
- J. R. Zimmerman, and M. R. Foster (1957). "Standardization of NMR high resolution spectra". J. Phys. Chem. 61 (3): 282–289. doi:10.1021/j150549a006.
- Robert Engel; Donald Halpern & Susan Bienenfeld (1973). "Determination of magnetic moments in solution by nuclear magnetic resonance spectrometry". Anal. Chem. 45 (2): 367–369. doi:10.1021/ac60324a054.
- P. W. Kuchel; B. E. Chapman; W. A. Bubb; P. E. Hansen; C. J. Durrant & M. P. Hertzberg (2003). "Magnetic susceptibility: solutions, emulsions, and cells". Concepts Magn. Reson. A 18: 56–71. doi:10.1002/cmr.a.10066.
- K. Frei & H. J. Bernstein (1962). "Method for determining magnetic susceptibilities by NMR". J. Chem. Phys. 37 (8): 1891–1892. Bibcode:1962JChPh..37.1891F. doi:10.1063/1.1733393.
- R. E. Hoffman (2003). "Variations on the chemical shift of TMS". J. Magn. Reson. 163 (2): 325–331. Bibcode:2003JMagR.163..325H. doi:10.1016/S1090-7807(03)00142-3. PMID 12914848.
- Wapler, M. C.; Leupold, J.; Dragonu, I.; von Elverfeldt, D.; Zaitsev, M.; Wallrabe, U. (2014). "Magnetic properties of materials for MR engineering, micro-MR and beyond". JMR. 242: 233–242. arXiv: . Bibcode:2014JMagR.242..233W. doi:10.1016/j.jmr.2014.02.005.
- R. E. Glick (1961). "On the Diamagnetic Susceptibility of Gases". J. Phys. Chem. 65 (9): 1552–1555. doi:10.1021/j100905a020.
- John F. Schenck (1993). "The role of magnetic susceptibility in magnetic resonance imaging: MRI magnetic compatibility of the first and second kinds". Medical Physics. 23: 815–850. Bibcode:1996MedPh..23..815S. doi:10.1118/1.597854. PMID 8798169.
- G. P. Arrighini; M. Maestro & R. Moccia (1968). "Magnetic Properties of Polyatomic Molecules: Magnetic Susceptibility of H2O, NH3, CH4, H2O2". J. Chem. Phys. 49 (2): 882–889. Bibcode:1968JChPh..49..882A. doi:10.1063/1.1670155.
- J. Heremans, C. H. Olk and D. T. Morelli (1994). "Magnetic Susceptibility of Carbon Structures". Phys. Rev. B. 49 (21): 15122–15125. Bibcode:1994PhRvB..4915122H. doi:10.1103/PhysRevB.49.15122.
- N. Ganguli & K.S. Krishnan (1941). "The Magnetic and Other Properties of the Free Electrons in Graphite". Proceedings of the Royal Society. 177 (969): 168–182. Bibcode:1941RSPSA.177..168G. doi:10.1098/rspa.1941.0002.
- Nave, Carl L. "Magnetic Properties of Solids". HyperPhysics. Retrieved 2008-11-09.
- R. Dupree & C. J. Ford (1973). "Magnetic susceptibility of the noble metals around their melting points". Phys. Rev. B. 8 (4): 1780–1782. Bibcode:1973PhRvB...8.1780D. doi:10.1103/PhysRevB.8.1780.
- S. Otake, M. Momiuchi & N. Matsuno (1980). "Temperature Dependence of the Magnetic Susceptibility of Bismuth". J. Phys. Soc. Jap. 49 (5): 1824–1828. Bibcode:1980JPSJ...49.1824O. doi:10.1143/JPSJ.49.1824. The tensor needs to be averaged over all orientations: .